1 downloads
0 Views
3MB Size

LETTER pubs.acs.org/NanoLett

Multispectral Plasmon Induced Transparency in Coupled Meta-Atoms Alp Artar,† Ahmet A. Yanik,† and Hatice Altug* Electrical and Computer Engineering Department, Boston University, Boston, Massachusetts 02215, United States

bS Supporting Information ABSTRACT: We introduce an approach enabling construction of a scalable metamaterial media supporting multispectral plasmon induced transparency. The composite multilayered media consist of coupled meta-atoms with radiant and subradiant hybridized plasmonic modes interacting through the structural asymmetry. A perturbative model incorporating hybridization and mode coupling is introduced to explain the observed novel spectral features. The proposed scheme is demonstrated experimentally by developing a lift-oﬀ-free fabrication scheme that can automatically register multiple metamaterial layers in the transverse plane. This metamaterial which can simultaneously enhance nonlinear processes at multiple frequency domains could open up new possibilities in optical information processing. KEYWORDS: Metamaterials, electromagnetically induced transparency, plasmons, plasmon hybridization, Fano resonances, strong coupling

E

lectromagnetically induced transparency (EIT), a spectrally narrow optical transmission window accompanied with extreme dispersion, results from quantum interference of multiple excitation pathways through short and long-lived resonances.1 Within this spectral window, dramatically slowed down photons and orders of magnitude enhanced nonlinearities can enable manipulation of light at few-photon power levels.2 Historically, EIT has been implemented in laser-driven atomic quantum systems. However, limited material choices and stringent requirements to preserve the coherence of excitation pathways in atomic systems have signiﬁcantly constrained the use of EIT eﬀect.3 Recent studies have revealed that EIT-like optical responses can be obtained classically using on-chip plasmonic and photonic nanoresonators.420 Much of the research eﬀort so far focused on isolated meta-atoms (either photonic or plasmonic) showing EIT-like eﬀect at a single resonance. On the other hand, metamaterial systems supporting EIT-like optical responses at multiple-spectral windows can simultaneously enhance multicolored photonphoton interactions and open up new possibilities in nonlinear optics and optical information processing.2123 In this Letter, we propose and demonstrate a novel approach based on coupled meta-atoms to construct a homogeneous and scalable medium supporting multispectral EIT-like eﬀect (plasmon induced transparency). The proposed structure consists of a two slot antenna based complementary metamaterial layers with a small gap (dielectric layer thickness) enabling strong near-ﬁeld interaction in between. Each planar metamaterial layer has bright (radiant) and dark (subradiant) plasmonic modes coupled through the structural asymmetry (s 6¼ 0) in an analogy to transition-allowed and -forbidden atomic orbitals coupled r 2011 American Chemical Society

through a common excited state.6 As shown in Figure 1b (blue curve), isolated meta-atoms on a single-layer metamaterial exhibit an EIT-like reﬂection10 with spectral features that are controlled by the artiﬁcial atomic orbitals (plasmonic modes). Once stacked in a multilayered structure (Figure 1b, black curve), presence of strong near-ﬁeld coupling between the meta-atoms causes splitting of the EIT resonances and leads to multispectral EIT-like behavior. The underlying physical principles for this phenomenon are related to plasmonic hybridization eﬀects24 and dark-bright mode couplings of the in-phase and out-phase hybridized states. To explain these novel spectral features, we introduce a perturbative model incorporating hybridization and mode coupling. Furthermore, we experimentally demonstrate the proposed scheme by developing a lift-oﬀ free fabrication scheme that can simultaneously register multiple metamaterial layers in the third dimension. In the following, we start by describing the perturbative model that provides insight into the physical processes involved in these structures. For the double layered metamaterial, a total Hamiltonian can be deﬁned as ~ ~0 þ H ~ 00 þ K ~ þΣ HT ¼ H ~ 00 are the 2 2 unperturbed Hamiltonians of ~ 0 and H Here, H the isolated metamaterial layers deﬁned in a basis set consisting of decoupled bright (dipolar) and dark (quadrupole) modes in the absence of a structural asymmetry (s 6¼ 0). The weak interactions between the bright and the dark modes Received: January 18, 2011 Revised: March 4, 2011 Published: March 25, 2011 1685

dx.doi.org/10.1021/nl200197j | Nano Lett. 2011, 11, 1685–1689

Nano Letters

LETTER

Figure 1. (a) Geometry of the multilayered metamaterial. Structure consists of two Au layers (30 nm thickness) that are separated by a dielectric (SiNx) layer (70 nm thickness). Each layer has a dipole and a quadrupole slot antenna (all slot antennas have 700 nm length, 100 nm width). The small in-plane separation between the dipolar and quadrupolar antennas is 50 nm on both sides and periods are 1200 nm on both x and y directions. Parameter s is deﬁned as the oﬀset of the dipolar antenna from the geometrical center of the structure. Blue arrows show the conﬁguration of the incident light. (b) Simulated reﬂection spectra for asymmetric (s 6¼ 0) single- and doublelayered structures are shown (with an oﬀset for clarity). Multispectral EIT-like response (in-phase and out-of-phase) is observable with double-layered metamaterial.

Figure 2. (a) Hybridization scheme for the dipolar mode. (b) Tuning of the spectra with the dielectric layer thickness is shown for the symmetric structure (s = 0). As the dielectric layer thickness reduces, splitting of energy between the hybrid modes increases. Single layer spectrum is shown with the blue dashed curve. Splitting energies (2εD) are 202, 260, 297 meV and energy oﬀsets (ΔD) are 60, 68, 78 meV for gap sizes (dielectric layer thicknesses) of 90, 70, 50 nm, respectively. (c) Charge distribution at the air/ metal interface (top view), demonstrating the dipolar mode excitation. This charge distribution is acquired from in-phase state |Dþæ of the multilayered structure; however the out-of-phase state |Dæ and also the single-layered dipolar state |D0æ have the exact same charge distribution (not shown). (d) Charge distributions of the hybrid dipolar modes acquired from a multilayered structure with a dielectric layer thickness of 50 nm (cross-sectional view) are shown at a position marked with the red dashed line in (c).

~ , when a are incorporated with the perturbative Hamiltonian K structural asymmetry is introduced (s 6¼ 0). Interactions between the two metamaterial layers are included through the strong near-ﬁeld coupling Hamiltonian Σ~. Accordingly, the total Hamiltonian for the coupled meta-atoms is given as

j1æ

j2æ

ÆD0 j " # H0 þ K Σ ÆQ0 j ¼ Σ H0 0 þ K0 ÆD0 0 j ÆQ0 0 j

~ ¼ Æ1j ~0 þ H ~ 00 þ K ~ þΣ HT ¼ H Æ2j

T Hhyb

ÆDþ j ^ T U ^ ¼ ÆD j ¼ U½H ÆQ þ j ÆQ j

jDþ æ

ED0 þ ΔD þ εD 6 6 0 6 6 k 4 0

in an orthogonal basis set consisting of 1 jD( æ ¼ pﬃﬃﬃ½jD0 æ ( jD0 0 æ 2

jD0 æ

ED0 6 6 k 6 6τ 4 inter, D ðχ0 Þ

jQ0 æ

jD0 0 æ

k E Q0 χ

τinter, D χ ED0 0 ðk0 Þ

τinter, Q

jQ0 0 æ χ0 τinter, Q k0 EQ0 0

3 7 7 7 7 5

ð1Þ

consideration in our analysis is that χ and χ0 , the cross couplings among the bright and dark modes, are weak and can be neglected. Validity of this assumption will be justiﬁed in the following by benchmarking our analytical relations with numerical simulations and experimental measurements. For a metamaterial system where the individual layers have identical structural characteristics, the Hamiltonian terms for both layers are identical (κ = κ0 , τinter,D/Q = τinter,D0 /Q0 , ED0/Q0 = ED0 0/Q0 0). After a simple rearrangement of the matrix elements and a unitary transformation, the total Hamiltonian can be rewritten as in

where |1æ and |2æ represent the top and bottom metamaterial layers, respectively. The eigenvalues of the bright (|D0æ) and the dark (|Q0æ) modes of the isolated metamaterials are deﬁned as ED0 and EQ0. For clarity, eigenstates and eigenvalues of the second layer are denoted with primes, even for structurally symmetric layers. κ and κ0 are due to the weak intralayer coupling among the dark and bright modes in each layer. τinter,D and τinter,Q are the strong interlayer coupling terms for the bright and dark modes, respectively. χ and χ0 are the cross couplings among the bright and dark modes of diﬀerent layers (interlayer). An important 2

2

ED0

jD æ

jQ þ æ

0 þ ΔD εD 0 k

k 0 þ Δ Q þ εQ 0

EQ0

jQ æ

EQ0

0 k 0 þ Δ Q εQ

1 jQ ( æ ¼ pﬃﬃﬃ½jQ0 æ ( jQ0 0 æ 2

ð3aÞ 1686

3 7 7 7 7 5

ð2Þ

ð3bÞ

dx.doi.org/10.1021/nl200197j |Nano Lett. 2011, 11, 1685–1689

Nano Letters

LETTER

~ (when ~0 þ H ~ 00 þ Σ diagonalizing the Hamiltonian HTs=0 = H the system is symmetric s = 0) in the strong coupling regime (|ED0 ED00 | , 2τinter,D and |EQ0 EQ00 | , 2τinter,Q). These hybrid eigenstate pairs are in-phase (þ) and out-of phase () superpositions of the isolated layer eigenmodes of the structurally symmetric multilayer system (s = 0). The associated energies of the dipolar hybrid modes are, E( D = ED0 þ ΔD ( εD, where the oﬀset term is ΔD = ÆD0|τinter,D|D0æ and the splitting term is εD = ÆD0|τinter,D|D00 æ (a similar set can be obtained for quadrupole modes). Since oﬀ diagonal terms in the transformed Hamiltonian HThyb are much weaker than the diagonal terms, the oﬀ-diagonal matrix elements κ and κ0 are treated as the elements of the perturbative Hamiltonian introduced by the structural asymmetry (s ¼ 6 0). Using the transformed Hamiltonian HThyb, a set of coupled Lorentzian oscillator relations can be derived in an analogy to atomistic EIT resonances. Initially, the hybridization of eigenstate pairs in the form of in-phase (þ) and out-of phase () superpositions of the isolated layer eigenmodes is shown in Figure 2 for the structurally symmetric multilayer system (s = 0 and κ = 0) using ﬁnite diﬀerence time-domain (FDTD) analysis. For a single-layered metamaterial, only the resonance dip corresponding to the excitation of the dipolar bright mode is observable in the reﬂection spectrum (Figure 2(b), dashed blue curve). For the double layered metamaterial, two resonance dips appear corresponding to in-phase and out-of-phase hybridized modes due to the degeneracy breaking as given in eq 3a (solid curves in Figure 2b). The mode energies and the splitting in between are controlled by the strength of the interlayer coupling of the metamaterial layers. As predicted by our Hamiltonian treatment, smaller gaps (dielectric layer thicknesses) lead to larger energy splittings as this coupling becomes stronger (Figure 2b). The in-phase and out-of-phase character of these hybridized states are also conﬁrmed with FDTD simulations showing cross-sectional charge distributions of the dipolar modes (Figure 2d). The in-phase hybrid mode is radiant as a result of its overall dipolar character. The radiant out-of-phase mode is harder to excite with respect to the in-phase mode, due to the partial cancellation of the dipolar moments of the subsequent layers. Nevertheless, resonance dip corresponding to the out-of-phase mode is still observable due to the retardation eﬀects (Figure 2b, solid curves). In Figure 2b, resonances due to hybridized quadrupolar modes are not observable, since any linear combination of the subradiant quadrupolar modes of the isolated structures is also subradiant. Structural symmetry must be broken for the excitation of these quadrupolar hybridized modes. Breaking the symmetry of the multilayered structure (s 6¼ 0) leads to near-ﬁeld coupling between the dark and bright modes (κ 6¼ 0) and results in the excitation of the dark modes with the perpendicularly incident light. Indirect excitation of these hybrid quadrupolar dark modes leads to multispectral EIT-like behavior (Figure 3 black curve). Charge distribution of the out-of-phase (OP) EIT resonance at the top surface (Figure 3a inset), indicates strong coupling of the external driving ﬁeld to this mode. A similar charge distribution is also observed for the inphase (IP) EIT resonance (not shown). Cross sectional charge distributions of the quadrupolar modes (Figure 3b) conﬁrm the in-phase and out-of-phase mode characters. Full spectral re2

ω ωþ þ iγþ D 6 þ 6 k 6 6 0 4 0

kþ ω ωþ δþ þ iγþ Q 0 0

Figure 3. (a) Asymmetric (s = 150 nm) and symmetric (s = 0 nm) double-layer EIT-like spectra. Two dips seen in the symmetric structure’s spectrum corresponds to hybrid dipolar modes as in Figure 2b. Asymmetric structure shows two EIT-like peaks at diﬀerent spectral positions. A model ﬁt based on Lorentzian harmonic oscillators is shown for the doublelayered structure (red dashed curve with κ = 12 THz, κþ = 23 THz),25 which traces the calculated spectra very well. A genetic search algorithm is implemented to extract the parameters using a least-squares sum ﬁt. Calculated group indices for the in-phase and out-of-phase modes are nþ g = 16, n g = 9.3. These values can be optimized by adjusting the coupling terms κ(. Inset shows the top view charge distribution at the air/metal interface for the out-of-phase EIT peak (in-phase EIT peak also shows the same distribution). Stronger excitation of the quadrupolar mode is shown. (b) Cross-sectional charge distributions of the quadrupolar antennas are shown at a position marked with the red dashed line in the inset. Hybridization of the quadrupolar resonance is shown.

sponse of the multilayered structure can be understood following our perturbative Hamiltonian approach. Here, a coupled Lorentzian oscillator model is derived from the transformed Hamiltonian HThyb in a similar way to the EIT concepts in atomic physics. In our analysis, the following three observations are employed. (i) Breaking of the structural symmetry (s 6¼ 0) results in weak near-ﬁeld coupling of the hybridized dark and bright modes, an eﬀect which can be incorporated to the unperturbative Hamiltonian (s = 0) with the perturbative terms κ and κ0 . (ii) There is no direct coupling between the in-phase and out-of-phase hybrid modes, due to the large energy diﬀerence in between (D( ( S Q-). (iii) Damping rates of the quadrupole (γ( Q ) and dipole (γD ) ( ( hybrid modes are small enough that the condition γQ , γD , ω( is satisﬁed. Here ω( are the resonant frequencies of the in-phase and ( out-of-phase hybrid pairs (ω( = E( D /p ≈ EQ /p). We can express all hybrid states in the form of |φæ = φ ~eiωt (where φ ( ( ~ is Q and D ) and denote the external driving ﬁeld as E0eiωt. Then, in agreement with the total Hamiltonian of the system, the following set of linear equations is obtained for the coupled Lorentzian oscillators

0 0 ω ω þ iγ D k 1687

2 3 32 þ 3 ~0 ~ 0 gþE D 7 6 7 7 6 7 76 6 ~þ 7 0 76 Q 7 ¼ 6 0 7 6 7 6 7 ~0 7 ~ 5 k 4g E 5 54 D ~ ω ω δ þ iγ 0 Q Q

ð4Þ

dx.doi.org/10.1021/nl200197j |Nano Lett. 2011, 11, 1685–1689

Nano Letters

LETTER

Here κ( values are the coupling parameters of the perturbative term for the in-phase and out-of-phase hybrid pairs, which are determined by the structural oﬀset “s”. δ( values are the small detuning of the frequencies of in-phase and out-of-phase hybrid ( ( mode pairs (δ( = (E( D EQ )/p). g values are the geometrical parameters that deﬁne the coupling eﬃciency of the dipolar hybrid modes (D() to the external ﬁeld. Equation 4 represents two coupled Lorentzian oscillator pairs corresponding to in-phase and out-of-phase hybridized modes of the whole structure. The external ﬁeld (E0) drives the bright modes in each meta-atom, which are subsequently coupled to the dark modes (through κ(). With these equations the amplitudes of the dipolar hybrid states (D() can be derived as ~( ¼ D

~0 ðω ω( δ( þ iγ( g ( E QÞ ( ( ( 2 ðω ω( þ iγ( D Þðω ω( δ þ iγQ Þ ðk Þ

ð5Þ

The complex amplitudes of the corresponding modes (given in eq 5) are directly proportional to the polarizability of the modes, which governs the spectral characteristics of the plasmonic structure. The overall spectral response is given by the superposition of these amplitudes. The close agreement between this analytical derivation and the FDTD analysis conﬁrms the validity of our perturbative model as shown in Figure 3a (dashed

Figure 4. Coupled three-level system model for multispectral plasmon induced transparency. Coupled meta-atoms have four states which form a ﬁve-level system with the continuum.

curve). The physical principles leading to multispectral EIT-like behavior can be equivalently observed in other structures. As an example, we implemented our approach with multilayered dolmen structures,6 and obtained a clear multispectral EIT-like behavior (see Supporting Information). Equation 5 is in close analogy to atomic physics, where the investigated atomic absorption cross section are given with a similar formula.1 This analogy allows us to illustrate multispectral EIT phenomena in our composite structure with ﬁve-level state diagram as shown in Figure 4. It is important to note that these eigenstates are strongly correlated, since they are a linear combination of the same basis sets (D0,Q0) as shown in the hybridization diagram in Figure 2a. Experimental veriﬁcation of this novel phenomenon is demonstrated using a lift-oﬀ free fabrication method that results in simultaneous patterning of multilayered slot antennas.26 In our fabrication scheme, we start with a free-standing membrane, which is patterned with nanoapertures using e-beam lithography and dryetching.27,28 Subsequent metal deposition on both sides with a highly directional e-beam evaporation results in multiple stacks that are automatically registered with respect to each other in the xyplane. Similarly, this fabrication scheme can be extended to fabricate devices with an even larger number of layers.29 Crosssectional scanning electron microscope (SEM) image of the ﬁnal structure shows negligible metal covering at the inner side walls (inset to Figure 5d). Spectral data collection is done with a Bruker IFS 66/s Fourier transform infrared (FTIR) spectrometer with a Hyperion 1000 IR microscope in reﬂection mode. In measurements obtained from the single-layered structure, a clear EIT-like spectral response is observed at a single frequency (∼100 THz, Figure 5c). On the other hand, experimental measurements obtained from the double-layered structure reveal two EIT peaks as predicted by the analytical relations (Figure 5d). The length of the dipolar slot antenna is 700 nm, and its width is 125 nm. The quadrupolar antenna lengths are 900 nm with a same width of 125 nm. The small in-plane separation between the dipolar and the quadrupolar antenna is 60 nm. The thicknesses of the deposited gold ﬁlms are 30 nm on both sides with a dielectric layer of 70 nm in between. A structural asymmetry (s) of 135 nm is introduced to enable the excitation of hybrid quadrupolar modes. In conclusion, we presented a method to extend the EIT-like phenomena to multiple spectral positions by tailoring the near-ﬁeld

Figure 5. (a) Illustration of the double-layered structure fabrication on a free-standing membrane. (b) SEM image of an array is shown. Reﬂection spectra of the symmetric (s = 0) and asymmetric (s 6¼ 0) for (c) single-layered and (d) double-layered structures are shown. A model ﬁt based on Lorentzian harmonic oscillators is shown for the double-layered asymmetric structure’s spectrum (red dashed curve with κ = 9.7 THz, κþ = 27.4 THz).30 The dipolar slot antenna length is 700 nm and the quadrupolar antenna lengths are 900 nm, all antenna widths are kept at 125 nm. The gap between the dipolar and quadrupolar antennas is 60 nm. Periods are 1200 nm on both x and y directions. Both Au layers are 30 nm with a 70 nm dielectric layer in-between. Inset in (d) shows the cross section image of the double-layered structure. Coverage of the sidewalls due to the metal deposition is minimal. 1688

dx.doi.org/10.1021/nl200197j |Nano Lett. 2011, 11, 1685–1689

Nano Letters coupling of meta-atoms in a multilayered metamaterial system. In particular, two near-ﬁeld interaction mechanisms make this phe~) nomena possible; (i) hybridization of plasmonic resonances (Σ ~ ). The and (ii) interaction between the bright and dark antennas (K method is demonstrated experimentally and theoretically with planar slot antenna based multilayered metamaterial systems. For experimental demonstration, a lift-oﬀ free fabrication scheme that can simultaneously register multiple metamaterial layers is introduced. The provided analytical investigations are kept general. Therefore, our method can be easily extended to other antenna geometries31 (see Supporting Information) as well as scaled to a larger number of metamaterial layers.

’ ASSOCIATED CONTENT

bS

Supporting Information. Additional information regarding electric ﬁeld distributions and enhancements at plasmon induced reﬂection peaks and multispectral plasmon induced transparency with nanoparticles. This material is available free of charge via the Internet at http://pubs.acs.org.

’ AUTHOR INFORMATION Corresponding Author

*E-mail: [email protected] Author Contributions †

These authors contributed equally

’ ACKNOWLEDGMENT This work is supported in part by NSF CAREER Award (ECCS-0954790), ONR Young Investigator Award, Massachusetts Life Science Center New Investigator Award, NSF Engineering Research Center on Smart Lighting (EEC-0812056), Boston University Photonics Center, and Army Research Laboratory. ’ REFERENCES (1) Boller, K. J.; Imamoglu, A.; Harris, S. E. Observation of electromagnetically induced transparency. Phys. Rev. Lett. 1991, 66, 2593–2596. (2) Harris, S. E.; Field, J. E.; Imamoglu, A. Nonlinear optical processes using electromagnetically induced transparency. Phys. Rev. Lett. 1990, 64, 1107–1110. (3) Liu, C.; Dutton, Z.; Behroozi, C. H.; Hau, L. V. Observation of coherent optical information storage in an atomic medium using halted light pulses. Nature 2001, 409, 490–493. (4) Yanik, M. F.; Fan, S. Stopping light all optically. Phys. Rev. Lett. 2004, 92, No. 083901. (5) N. Papasimakis, N.; Fedotov, V. A.; Zheludev, N. I.; Prosvirnin, S. L. Metamaterial analog of electromagnetically induced transparency. Phys. Rev. Lett. 2008, 101, No. 253903. (6) Zhang, S.; Genov, D. A.; Wang, Y.; Liu, M.; Zhang, X. Plasmoninduced transparency in metamaterials. Phys. Rev. Lett. 2008, 101, No. 047401. (7) Liu, N.; Langguth, L.; Weiss, T.; Kastel, J.; Fleischhauer, M.; Pfau, T.; Giessen, H. Plasmonic analogue of electromagnetically induced transparency at the Drude damping limit. Nat. Mater. 2009, 8, 758–762. (8) Shvets, G.; Wurtele, J. S. Transparency of magnetized plasma at the cyclotron frequency. Phys. Rev. Lett. 2002, 89, No. 115003. (9) Luk’yanchuk, B.; Zheludev, N. I.; Maier, S. A.; Halas, N. J.; Nordlander, P.; Giessen, H.; Chong, C. T. The Fano resonance in plasmonic nanostructures and metamaterials. Nat. Mater. 2010, 9, 707–715.

LETTER

(10) Liu, N.; Weiss, T.; Mesch, M.; Langguth, L.; Eigenthaler, U.; Hirscher, M.; Sonnichsen, C.; Giessen, H. Planar metamaterial analogue of electromagnetically induced transparency for plasmonic sensing. Nano Lett. 2009, 10, 1103–1107. (11) Zia, R.; Schuller, J.; Chandran, A.; Brongersma, M. Plasmonics: the next chip-scale technology. Mater. Today 2006, 9, 20–27. (12) Hao, F.; Sonnefraud, Y.; Dorpe, P. V.; Maier, S. A.; Halas, N. J.; Nordlander, P. Symmetry breaking in plasmonic nanocavities: Subradiant LSPR sensing and a tunable Fano resonance. Nano Lett. 2008, 8, 3983–3988. (13) Verellen, N.; Sonnefraud, Y.; Sobhani, H.; Hao, F.; Moshchalkov, V. V.; Dorpe, P. V.; Nordlander, P.; Maier, S. A. Fano resonances in individual coherent plasmonic nanocavities. Nano Lett. 2009, 9, 1663– 1667. (14) Mirin, N. A.; Bao, K.; Nordlander, P. Fano resonances in plasmonic nanoparticle aggregates. J. Phys. Chem. A 2009, 113, 4028. (15) Fan, J. A.; Wu, C.; Bao, K.; Bao, J.; Bardhan, R.; Halas, N. J.; Manoharan, V. N.; Nordlander, P.; Shvets, G.; Capasso, F. Selfassembled plasmonic nanoparticle clusters. Science 2010, 328, 1135– 1138. (16) Lassite, J. B.; Sobhani, H.; Fan, J. A.; Kundu, J.; Capasso, F.; Nordlander, P.; Halas, N. J. Self-assembled plasmonic nanoparticle clusters. Nano Lett. 2010, 10, 3184–3189. (17) Hao, F.; Nordlander, P.; Sonnefraud, Y.; Dorpe, P. V.; Maier, S. A. Tunability of subradiant dipolar and Fano-type plasmon resonances in metallic ring/disk cavities: implications for nanoscale optical sensing. ACS Nano 2009, 3, 643–652. (18) Hentschel, M.; Saliba, M.; Vogelgesang, R.; Giessen, H.; Alivisatos, A. P.; Liu, N. Transition from isolated to collective modes in plasmonic oligomers. Nano Lett. 2010, 10, 2721–2726. (19) Evlyukhin, A. B.; Bozhevolnyi, S. I.; Pors, A.; Nielsen, M. G.; Radko, I. P.; Willatzen, M.; Albrektsen, O. Detuned electrical dipoles for plasmonic sensing. Nano Lett. 2010, 10, 4571–4577. (20) Mukherjee, S.; Sobhani, H.; Lassiter, J. B.; Bardhan, R.; Nordlander, P.; Halas, N. Fanoshells: Nanoparticles with built-in Fano resonances. Nano Lett. 2010, 10, 2694–2701. (21) Kekatpure, R. D.; Barnard, E. S.; Cai, W.; Brongersma, M. Phase-coupled plasmon-induced transparency. Phys. Rev. Lett. 2010, 104, No. 243902. (22) Xu, Q.; Sandhu, S.; Povinelli, M. L.; Shakya, J.; Fan, S.; Lipson, M. Experimental realization of an on-chip all-optical analogue to electromagnetically induced transparency. Phys. Rev. Lett. 2006, 96, No. 123901. (23) Lukin, M. D.; Imamoglu, A. Nonlinear optics and quantum entanglement of ultraslow single photons. Phys. Rev. Lett. 2000, 84, 1419–1422. (24) Prodan, E.; Radloﬀ, C.; Halas, N. J.; Nordlander, P. A hybridization model for the plasmon response of complex nanostructures. Science 2003, 302, 419–422. (25) Other used model parameters are, ωþ/ω = 128/57 THz, δþ/ δ = 0.9/0.8 THz, γQþ/γQ = 8.32/6.1 THz, γDþ/γD = 30.7/ 17.7 THz. (26) Yanik, A. A.; Huang, M.; Artar, A.; Chang, T. Y.; Altug, H. Integrated nanoplasmonic-nanoﬂuidic biosensors with targeted delivery of analytes. Appl. Phys. Lett. 2010, 96, No. 021101. (27) Aksu, S.; Yanik, A. A.; Adato, R.; Artar, A.; Huang, M.; Altug, H. High-throughput nanofabrication of infrared plasmonic nanoantenna arrays for vibrational nanospectroscopy. Nano Lett. 2010, 10, 2511–2518. (28) Artar, A.; Yanik, A. A.; Altug, H. Fabry-Perot nanocavities in multilayered plasmonic crystals for enhanced biosensing. Appl. Phys. Lett. 2009, 95, No. 051105. (29) Valentine, J.; Zhang, S.; Zentgraf, T.; Ulin-Avila, E.; Genov, D. A.; Bartal, G.; Zhang, X. Three-dimensional optical metamaterial with a negative refractive index. Nature 2008, 455, 376–379. (30) Other used model parameters are, ωþ/ω= 131/50 THz, δþ/δ = 14.9/4.8 THz, γQþ/γQ = 12.19/4.49 THz, γDþ/γD = 45.7/11.9 THz. (31) Cubukcu, E.; Kort, E. A.; Crozier, K. B.; Capasso, F. Plasmonic laser antenna. Appl. Phys. Lett. 2006, 89, 093120-22. 1689

dx.doi.org/10.1021/nl200197j |Nano Lett. 2011, 11, 1685–1689